Reference:Reference: PolymerPolymer PropertiesProperties
Viscosity Viscosity Terms η rel is determined by the ratio t/t0, where (t) is the outflow time of a given volume of solution and 0(t) is the outflow time of the equivalent volume of pure solvent. Values are commonly determined with a capillary viscometer. Other viscosity terms are defined in Table I.
Table I: Definition of Viscosity Terms
IUPAC Name Common Name Definition Symbol Units η η η Viscosity ratio Relative viscosity / 0 rel dimensionless η/η η Specific viscosity Specific viscosity 0 -1 sp dimensionless η η Viscosity number Reduced viscosity sp /c red deciliter/gram η η Logarithmic viscosity number Inherent viscosity In rel /c inh deciliter/gram Limiting viscosity number Intrinsic viscosity lim (η /c) [η] deciliter/gram c ← 0 sp lim (ln η /c) c ← 0 rel Absolute viscosity P Poise (dynes · s/cm) Pa · s Pascal · second (Newton · s/m2) Kinematic Viscosity St Stokes (m2/s) Conversion factor: η(Poise) = η(Stoke) x density (g/cm3)
Viscometer Comparison for NEWTONIAN Liquids The chart1 below is intended to be an aid in comparing viscometer measurements of Newtonian liquids by referencing to absolute and kinematic viscosity.
Mobilometer 100g 10cmsec.
Ford 4 sec.
Ford 3 sec.
Saybolt Universal sec.
Saybolt Furol sec.
Redwood Standard "1 sec.
Gardner Holts cks.
Zahn 5 sec.
Zahn 3 sec.
Kreb Stormer 200G K.U.
Stormer Cyl. 150G sec.
1 Reprinted with permission from Brookfield Engineer ing Laboratories, Inc., Stoughton, MA, U.S.A.
50 Polymer Products from Aldrich a Reference:Reference: PolymerPolymer PropertiesProperties
Viscosity - Molecular Weight Relationships Mark-Houwink-Sakurada Equation:
a [η]=KM...... Eq. 1 where: [η] = intrinsic viscosity, K and a = constants, dependent on the polymer, solvent, and temperature Caution must be exercised in applying this relationship since the K value is greatly influenced by the molecular weight distribution of the polymer sample used in the determination. Within a giv en series of polymer homologs , [η] increases with the molecular w eight M. This is illustr ated in Table I f or poly(dimethylsiloxane). The molecular weight of polymers such as poly(vinyl chloride) and poly(vinyl pyrrolidone) are often reported in terms of the Fikentscher K-value, derived from a solution viscosity (see Glossary under K-value) which should not be confused with the constant K of the Mark-Houwink-Sakurada equation (1). The relationship between the intrinsic viscosity, K-value, and approxi- mate molecular weight is illustrated in Tables II and III for PVC and PVP, respectively.
ηηη Table I: [ ] - Mw relationship for Table II: Relationship between intrinsic viscosity, poly(dimethylsiloxane), trimethylsilyl terminated1 K-value and approximate molecular weight for poly(vinyl chloride)2
Viscosity, cSt @ 25°CMw Intrinsic K Value 1.0 240 viscosity,[η] 1% in Cyclohexanone M M 2.0 400 η w 5.0 800 0.52 50 20,000 40,000 10 1,300 0.67 57 27,500 55,000 50 4,000 0.92 67 41,000 82,500 200 9,500 1.08 72 50,000 101,000 500 17,000 1.30 79 62,500 123,500 1000 28,000 1.60 87 81,000 168,000 10,000 63,000 2 Perkins, G.G.A. et.al., J. of Vinyl Technology, 1993, 108,15. 100,000 140,000
1 Mw values are approximate and should be used as a guide for the estimated molecular weight.
Table III: Relationship of viscosity, K-Value, and approximate molecular weight for poly(vinylpyrrolidone) (PVP)3
Viscosity in water K Value
cSt (%PVP) range Mη M w 7(20) 13-19 10,000 12,000 25(20) 26-34 40,000 55,000 50(10) 50-62 220,000 400,000 400(10) 80-100 630,000 1,280,000 7000(10) 115-125 1,450,000 2,800,000
3 GAF(ISP) Technical Bulletin 2302-203 SM-1290, “PVP polyvinylpyrroli- done Polymers”, 1990. a The Link to All Your Polymer Needs 51